1 Aus dem Max-Planck-Institut für Kolloid- und Grenzflächenforschung Synthese und Kolloidale Eigenschaften neuartiger Blockcopolymere mit β-dicarbonyl Einheiten Synthesis and Colloidal Properties of a Novel Type of Block Copolymers bearing β-dicarbonyl Residues Dissertation Zur Erlangung des akademischen Grades Doktor der Naturwissenschaften (Dr. rer. nat.) in der Wissenschaftsdisziplin Physikalische Chemie eingereicht an der Mathematisch-Naturwissenschaftlichen Fakultät der Universität Potsdam von Theodora Krasia aus Nikosia, Zypern Golm, im April 2003
2 Die vorliegende Arbeit entstand in der Zeit von ctober 2000 bis April 2003 am Max- Planck-Institut für Kolloid- und Grenzflächenforschung, Golm. Gutachter: - Prof. Dr. M. Antonietti - Dr. habil. H. Cölfen - Prof. Dr. U. S. Schubert Tag der mündlichen Prüfung:
3 Vorstellungskraft ist wichtiger als Wissen. The power of imagination is more important than knowledge. Albert Einstein, Wissenschaftler, To my family in Cyprus and here in Germany...
4 Table of Contents 1 Abstract 1 2 Introduction Block copolymers Phase separation behaviour of block copolymers Micellisation Living /Controlled polymerisation Anionic polymerisation Group transfer polymerisation (GTP) Reversible addition-fragmentation chain-transfer polymerization(raft) Functionalised polymers with metal complexing segments Characterisation methods Gel permeation chromatography Scattering methods Dynamic light scattering Static light scattering Microscopy techniques Atomic force microscopy Scanning electron microscopy Analytical ultracentrifugation Double-Jet method Results and discussion Synthesis and characterisation of amphiphilic block copolymers with β-dicarbonyl segments Hydrophobic block copolymers with β-dicarbonyl segments by GTP.. 35
5 4.1.2 Hydrophilic block copolymers with β-dicarbonyl segments by Anionic polymerization Homo and block (co)polymers with β-dicarbonyl segments by RAFT Synthesis of well-defined paemas Synthesis of well-defined block copolymers based on AEMA Investigation of the aggregation behaviour of hydrophobic block copolymers with β-dicarbonyl segments in organic media Micellisation behaviour in selective solvents H-bond interactions between adjacent β-dicarbonyl segments in paema: Aggregation behaviour of amphiphilic block copolymers with a β-dicarbonyl segment in the presence of inorganic metal ion salts in solution Complexation of FeCl. 3 6H 2 in hydrophobic media via the keto form of β-dicarbonyl units Complexation of FeCl. 3 6H 2 and Pd(Ac) 2 in hydrophobic media via the enolate form of β-dicarbonyl units Shape transition upon complexation in different solvent systems Formation of sheet-like superstructures from micellar solutions of pbuma-bpaema loaded with FeCl. 3 6H Water-soluble block copolymers with β-dicarbonyl ligating segments: Biomineralisation applications Preface Effect of paee-b-pe block copolymers on the nucleation behaviour of calcium carbonate in water Summary and utlook Experimental part Experimental techniques Solvents and reagents.. 99
6 6.3 Synthesis Monomer synthesis (TMSHEMA) Polymer synthesis Synthesis by GTP pbuma-b-ptmshema pbuma-b-phema pbuma-b-paema Synthesis by anionic polymerisation pb-b-pe phee-b-pe paee-b-pe Synthesis by radical polymerisation methods paema (free radical polymerisation) paema (RAFT polymerisation) pmma-b-paema (RAFT) paema-b-pbuma (RAFT) paema-b-pbua (RAFT) paema-b-pnipam (RAFT) Appendix Abbreviations Acknowledgements Literature.. 135
7 CHAPTER 1 Abstract The present work is dealing with the first synthesis and characterisation of amphiphilic diblock copolymers bearing β-dicarbonyl (acetoacetoxy) chelating residues. Polymers were obtained by Group Transfer Polymerisation (GTP)/acetoacetylation and controlled radical polymerisation techniques (RAFT). Different micellar morphologies of poly(n-butyl methacrylate)-block-poly[2- (acetoacetoxy)ethyl methacrylate] (pbuma-b-paema) were observed in cyclohexane as a selective solvent. Depending on the block length ratio, either spherical, elliptical, or cylindrical micelles were formed. The density of the polymer chains at the core/corona interface is considerably higher as compared to any other strongly segregating system reported in the literature. It is demonstrated that there are H-bond interactions existing between acetoacetoxy groups, which increase the incompatibility between block segments. In addition, such interactions lead to the formation of secondary structures (such as β-sheets or globular structures) and larger superstructures in the micrometer length scale. Block copolymers were also used to solubilise metal ion salts of different geometries and oxidation states in organic media, in which are otherwise insoluble. Sterically stabilised colloidal hybrid materials are formed, i.e. monodisperse micelles having the metal ion salt incorporated in their core upon complexation with the ligating paema block, whereas pbuma forms the solvating corona responsible for stabilisation in solution. Systematic studies show that the aggregation behaviour is dependent on different factors, such as the tautomeric form of the β-dicarbonyl ligand (keto/enol) as well as the nature and amount of added metal ion salt.
8 INTRDUCTIN 2 CHAPTER 2 Introduction 2.1 Block copolymers Block copolymers are macromolecules consisting of at least two blocks of constitutionally and/or configurationally different monomeric units, for example A m -B n, A m -B n -A m etc. The different blocks are connected together via covalent bonds 1. Unlike other copolymers, they retain many of the physical characteristics of the homopolymer sections. According to the number of different blocks incorporated in a block copolymer, these materials are classified in di-, tri-, or multi- block copolymers. Usually, the different blocks are thermodynamically immiscible due to their different polarity. A special class of block copolymers in which hydrophobic and hydrophilic segments are incorporated, similar to low molecular weight surfactant molecules is the so called Amphiphilic Block Copolymers. The word derives from the greek αµϕι [amphi = both] and ϕιλος [Philos = friend]. This amphiphilic character causes a microphase separation, a phenomenon in which similar blocks of different block copolymer molecules aggregate and form different morphologies (see 2.2). The latter are mainly governed by the relative spatial requirements of the blocks 1. Two examples are presented in Figure 2.1. Lamellae structures, where a layer of one block faces another layer of the same type 1 and spherical domains of one block in a matrix of another can be formed. Such separation occurs not only at a water/oil interface but also at interfaces such as polymer/polymer (blends) metal/polymer and others 2. a b Figure 2.1: Arrangement of A blocks ( ) and B blocks ( ) in diblock and triblock copolymers: (a) Formation of spherical domains of A-blocks in a continuous matrix of B blocks in an ABA triblock copolymer and (b) Lamellar structure of AB diblock copolymers with equal block volumes 1.
9 INTRDUCTIN 3 Depending on the nature of the monomers, the number and lengths of the block segments, as well as the chain architecture (linear, branched, graft, stars etc.), block copolymers can exhibit a wide range of interesting properties. Additionally, their ability to solubilise in different solvents and the presence of functional groups, make them versatile in many industrial applications. Block copolymers can be synthesised either via coupling reactions occurring between different homopolymer segments with functional end-groups 3, or sequential polymerisation of different monomers 4. To the latter and most commonly used, belong different living, controlled polymerisation techniques such as anionic 5, cationic 6,7,8,9, radical 10,11 and coordination polymerisation 12, Phase separation behaviour of block copolymers Mixing two polymers most commonly results in total phase separation on a macroscopic level. This phenomenon can be qualitatively explained in terms of the reduced combined mixing entropy of two different types of polymer chains 14. In a block copolymer, due to the presence of a covalent bond between the two blocks, microphase separation occurs. The formation of microdomains is attributed to the fact that one block resides in one phase, whereas the second one in the neighbouring phase. The covalent bond between the two blocks plays the role of the interface in this microphase-separated system 15. The selfassembly behaviour of amphiphilic block copolymers in organic and aqueous media depends on the chemical composition and block lengths, as well as temperature, concentration, and interfacial energy. Hence, a number of different structures and morphologies can be obtained such as micelles of different shapes (spherical, cylindrical, etc., see 2.3), ordered continuous morphologies (lamellae, ordered cylinders) or bicontinuous structures 2. An overview of the most common structures formed by diblock copolymers is presented in Figure
10 INTRDUCTIN 4 Spherical micelle H B Cylindrical micelle Vesicle G L Figure 2.2: Common morphologies of microphase-separated block copolymers: Body centred cubic packed spheres (B), hexagonally ordered cylinders (H) gyroid (G), lamellar (L), cylindrical micelles, vesicles, spherical micelles etc 2. There are three basic parameters which determine the size (usually nm) and shape of the microdomains formed by an AB diblock copolymer 2 : (i) (ii) (iii) The degree of polymerisation (N) which is equal to the sum of DPs of the two blocks, The composition of each block, i.e. f A = N A /N and f B = N B /N and The Flory - Huggins interaction parameter χ AB, which characterises polymer/polymer interactions. (in bulk). The Flory Huggins parameter depends on temperature. This dependence is approximately given by: χ A + B/T (2.1) A and B are constants which differ from system to system 1.
11 INTRDUCTIN 5 In bulk, the tendency for microphase separation depends on the term χn, in which enthalpic and entropic contributions are included 16. Small values of this parameter ( 10), describe a non-ordered system in which the polymer blocks are highly miscible with each other, i.e the interface between them is large. This is known as the Weak Segregation Limit (WSL) 17. The second regime of phase behaviour is referred to as the Strong Segregation Limit (SSL) when χn>10. In this case, mixing of the different blocks is energetically unfavourable, leading to the development of small interfaces between the different blocks, thus phase separation. It is in this region where well known morphologies such as lamellae, body centred cubic packed spheres (BCC) and hexagonally ordered cylinders (HEX) are stable 2. Furthermore, Khoklov et al. 18 have named a new regime Super Strong Segregation Limit (SSSL) in the cases where χn>>10. The various bulk block copolymer morphologies can be presented on a phase diagram of χn versus the composition of a specific block, f. An example of such a diagram derived from theoretical calculations by Matsen and Bates 19, 20 is presented in Figure 2.3. Figure 2.3: Calculated phase diagram for block copolymers: L: Lamellae; H: Hexagonally ordered cylinders; Q Im3m : Body centred cubic packed spheres; Q Ia3d : Gyroid; CPS: Cubic packed spheres; DIS: Disordered phase 19,20.
12 INTRDUCTIN Micellisation The phenomenon of micellisation of block copolymers, received much attention in the last decades and up to date, numerous experimental and theoretical investigations have been reported on this subject 21,22. Several reviews on micellisation phenomena of non-ionic block copolymers in non-aqueous 23 and aqueous 24,25 media as well as on ionic block copolymer micelles 26,27 have been published. In selective solvents, amphiphilic block copolymers form aggregates consisting of rather dense cores of the insoluble blocks, surrounded by diffuse outer shells (coronas) of the soluble ones 28 (Figure 2.4). Figure 2.4: Schematic representation of a spherical block copolymer micelle showing a dense core and a diffuse corona. Even though polymeric and low molecular weight amphiphilic systems resemble each other in many aspects, such as the formation of different micellar structures (spherical, cylindrical, etc.), polymeric amphiphiles can generate microphases which are thermodynamically and kinetically more stable. Due to this high stability, such systems can be used in a wide range of applications such as emulsion polymerisation, colloid stabilisation, drug delivery, or as microreactors 17. Micelle formation of block copolymer systems is determined by three main parameters: The respective block lengths N A and N B and the Flory Huggins parameter, χ. Unlike in bulk, here χ considers both polymer/polymer and polymer/solvent interactions. Further parameters of interest are the statistical segment length, l k and the monomer volume, v o. Assuming that the micellar core is mostly constructed of A blocks and the corona is rich in B blocks, three types of micellar structures can exist, depending on the relative block lengths of N A and N 17 B :
13 INTRDUCTIN 7 - if N A <<N B, meaning that the corona is much larger than the core, then the size of the corona is approximately equal to the size of the micelle. This type is called hairy micelle (Figure 2.5(a)). - In the opposite situation, where N A >>N B, the core is much larger than the corona and a crew cut micelle is formed. (Figure 2.5 b). (a) Figure 2.5: Schematic representation of (a) a hairy micelle and (b) a crew cut micelle. (b) The third class of micelles is called amphiphilic micelles. The main characteristic of this micellar type is the large interaction parameter χ. As already mentioned in 2.2, the term χn can be used to describe the tendency for microphase separation in bulk. In solution, if the interaction parameter χ AB (corresponding to interactions between the two blocks), is approximately equal to the one which describes the polymer/solvent interactions of the one block (χ AS ) and these are much larger than that of the polymer/solvent interactions of the second block, (χ BS ), then χn can serve as a parameter for characterising the thermodynamic state 17. In the SSSL regime (χn>>10), the core consists basically of A blocks, the corona consisting of B domains is swollen with solvent, whereas in the solvent phase no block copolymers are present 17. In conclusion, in the term Amphiphilic micelles both types of micelles, (hairy and crew cut) can be included as long as strong segregation is involved. The three different micellar types exhibit characteristic scaling relations with the aggregation number Z, (i.e the number of individual block copolymer chains per micelle) and the radius R 17 :
14 INTRDUCTIN 8 Hairy Micelle Z N A 4/5 N A <<N B R N A 3/5 Crew cut Micelle Z N A 1 N A >>N B R N A 2/3 Amphiphilic Micelle Z N A 2 large χ R N A 1 Förster and co-workers 17 have prepared a series of non-ionic amphiphilic diblock copolymers of the type poly(styrene)-b-poly(4-vinylpyridine). These form micelles in toluene, a selective solvent for the ps block, the size and shape of which were characterised by light scattering and electron microscopy. They have shown that for these systems, Z exhibits a scaling relation with N, the polymerisation degree for each block: Z N P4VP 2 N PS -0.8 (2.2) Figure 2.6: Aggregation numbers Z as a function of N A and N B for diblock and triblock copolymer systems 17,29 (empty data points) as well as ionic and non-ionic surfactants (solid data points) 30. As shown in the above figure, this behaviour is comparable to that of strongly segregated block copolymer systems as well as low molecular weight ionic and non-ionic surfactants.
15 INTRDUCTIN Living /Controlled Polymerisation ne of the most important aims of synthetic polymer chemistry is the achievement of control, not only on molecular weights (MW) and molecular weight distributions (MWD) of the polymer chains, but also on their compositions and architectures. Living polymerisation appears to be the most suitable and convenient method for this purpose, since it proceeds in the absence of chain transfer or irreversible termination reactions 5. Most of the chain ends are in a dormant inactive form found in rapid equilibrium with the active species. Usually, initiation and exchange equilibrium reactions between active/inactive species are fast compared to propagation, thus resulting in polymers with controlled molecular weights and narrow molecular weight distributions (Poisson). Molecular weights can be theoretically determined by the molar ratio of monomer to initiator 5. Anionic and Group Transfer Polymerisation (GTP) are two important examples for living polymerisation methods of methacrylates. Another controlled polymerisation technique is the radical Reversible Addition-Fragmentation Chain-Transfer Polymerisation (RAFT). Here, the controlled character is conferred by the presence of dithiocarbonyl compounds, which serve as chain transfer agents (CTA) 31. These three polymerisation processes were used in the synthesis of homo and block copolymers reported in this work Anionic Polymerisation In 1956, Szwarc 32 first described living anionic polymerisation. In such systems, stable active anionic chain ends are generated via the addition of the initiator across the double bond of a monomer. These can be used for synthesising functionalised, block, star and graft copolymers. Additionally, anionic polymerisation ensures control over molecular weights and molecular weight distributions and provides the possibility for controlling stereoselectivity. The degree of polymerisation, DP, is determined from the ratio of monomer concentration, [M] o to the concentration of active species, [P*], and it is proportional to the percentage of monomer consumption, x. The concentration of active species depends on the initiator efficiency, f i and the initial concentration of the initiator, [I] o. Therefore, DP can be expressed as:
16 INTRDUCTIN 10 DP = x[ M ] o x[ M ] o = [ P *] 0 f i  I o [ M ] x = 1 - [ M ] o (2.3) (2.4) where [M] o corresponds to the initial and [M] to the final monomer concentration. For an ideal living polymerisation process, all chains are initiated essentially at the same moment and all of them grow at the same rate until all monomer is consumed 33. In such case, MWD is very narrow and follows a Poisson-distribution as depicted in Figure 2.7. n x corresponds to the number of chains with DP = x and N to the total number of chains. n x /N DP Figure 2.7: Poisson distribution of simultaneously initiated and propagated polymer chains in an ideal living polymerisation process. The polydispersity index, (PDI), is determined from equation 2.5 as: PDI = M w DP = 1 + ( ) 2 M n DP , for DP >>1 (2.5) DP In order for living anionic polymerisation to proceed without termination, inert atmosphere or vacuum techniques are required to exclude moisture, oxygen and carbon dioxide 5. Furthermore, factors such as the proper choice of initiator, solvent, temperature, counterion and additives can affect the way in which anionic polymerisation of a particular monomer proceeds 5. Alkali-metal suspensions, alkyl or aryllithium reagents, organic radical ions or Grignard reagents are usually used as initiators. Typical monomers that can be polymerised
17 INTRDUCTIN 11 anionically are styrene, (meth)acrylates, 1,3-dienes, vinylpyridine, oxiranes, lactones and cyclic siloxanes Group Transfer Polymerisation (GTP) In 1983, Webster and co-workers introduced a silicon-mediated polymerisation of acrylic esters 34, which was named Group Transfer Polymerisation (GTP). This new polymerisation process displayed features characteristic of a living polymerisation at room temperature 35. The monomers used in this polymerisation method are vinyl monomers containing carbonyl or cyano groups in the side chain. Methacrylates are considered to be the most appropriate monomer type for GTP. As catalysts, difluoro ions, F - 2, or oxyanions, C -, are used. In the present work tetrabutylammonium bibenzoate (TBABB) served as the catalyst, and a silyl ketene acetal, 1-methoxy-1-trimethylsiloxy-2-methylprop-1-ene (MTS) was used as the initiator. GTP involves a sequential Mukiyama-Michael addition of silyl ketene acetal with alkyl (meth)acrylate in the presence of a small amount of a nucleophilic or Lewis acid catalyst 36. The name Group Transfer Polymerisation was suggested because early studies on the reaction mechanism indicated that the trimethylsilyl group coordinated with a pentacoordinated siliconate anionic catalyst, was transferred from the initiator or propagating chain-end to the carbonyl oxygen of the incoming monomer (Figure 2.8) 37. Si(Me) 3 Si(Me) 3 Me + Me Nu - THF, 25 o C Me Me xmma H CH 3 H x Me Me Me x+1 + CH3 Si(Me) 3 Me Me Si(Me) 3 Figure 2.8: Nucleophile assisted GTP of MMA 38. The way in which a nucleophilic and a Lewis acid catalyst participate in the polymerisation process is different. Many proposals concerning GTP polymerisation mechanism, depending on the type of catalyst used were reported. As already mentioned, Webster and Sogah
18 INTRDUCTIN 12 proposed that during propagation, an intramolecular transfer of pentacoordinated siliconate from a chain-end to the carbonyl group of an incoming monomer takes place via an eight membered-transition state (associative-intramolecular GTP mechanism). However, Mai and Müller 39,40 proposed a modified associative mechanism based on kinetic studies. This involved two steps: At first, the monomer adds to the α carbon of the pentacoordinated siliconate chain-end. Subsequently, the silyl group migrates to the carbonyl oxygen of the monomer. A dissociative GTP mechanism in which pentacoordinated siliconate dissociates to the ester enolate anion was also proposed 41. The latter reacts with monomer and forms reversibly a silyl ketene acetal end-group. It is believed that the propagating ester enolate anions undergo a faster silicon exchange between propagating chain ends. In this case, control over molecular weights is ensured by the ratio of monomer to initiator rather than monomer to catalyst 38. The proposed associative and dissociative GTP mechanisms are presented in Figure 2.9. Si(Me) 3 Me + Nu - Si(Me) 3 Me Nu - MMA - Me Nu Si(Me) 3 Me Associative-intramolecular GTP nmma pmma pentacoordinate siliconate intermediate - + NuSiMe 3 Me Dissociative-intermolecular GTP Figure 2.9: Associative and dissociative transfer mechanisms of MMA in GTP 38. Group Transfer Polymerisation has many advantages. Firstly, it proceeds rapidly and provides quantitative polymer yields. As mentioned before, it provides good control over the molecular weights and molecular weight distributions. Furthermore, in contrast to other polymerisation methods, which take place at very low temperatures, GTP occurs at ambient temperature. This point is quite important, since no special experimental techniques for temperature control during polymerisation are required 42. The polymerisation degree, as in anionic polymerisation, is determined from the molar ratio of monomer to initiator. In addition to the synthesis of homopolymers, it can be also used to produce block, stars and network copolymer architectures. However, GTP has some disadvantages. With this method,
19 INTRDUCTIN 13 molecular weights over 50,000 g/mol cannot be obtained. This explains the broad molecular weight distributions observed for high molecular weight polymers and also the lack of quantitative polymerisation yields. A second disadvantage is that a wide range of monomers is excluded from the list of those capable of being polymerised by GTP Reversible Addition-Fragmentation Chain-Transfer Polymerisation (RAFT) RAFT represents a new versatile polymerisation technique, which allows for the preparation of well-defined polymers with functionalised end-groups 11,43, 44. The process shows many of the characteristics of controlled polymerisations such as: - narrow molecular weight distributions (usually <1.2; sometimes <1.1) 11 - linear molecular weight conversion profile - preparation of block copolymers and other complex architectures such as stars, 45, 46, 47, 48 branched or block copolymer networks by the addition of a second monomer - control over the molecular weight. The DP can be easily derived using equation 2.6: x*[m] o /[CTA] o (2.6) where x is the monomer conversion, [M] o the initial monomer concentration and [CTA] o the initial concentration of the chain transfer agent. - compatibility with a wide range of monomers (including functional monomers containing for example acid, acid salt, hydroxy or tertiary amino groups) and reaction conditions (no particular limitations on solvent or reaction temperature) polymerisations can be performed in bulk, solution, emulsion or suspension. The controlled character of this free radical polymerisation method is attributed to the presence of dithiocarbonyl compounds (Figure 2.10), which mediate the polymerisation via a reversible chain transfer process 49. Usually, azo or peroxy initiators are employed. z S S R1 Figure 2.10: General chemical structure of dithiocarbonyl compounds used as CTA in RAFT.
20 INTRDUCTIN 14 For the achievement of high chain transfer constants, group Z should be able to activate the C=S double bond. Aryl and alkyl groups are suitable for this purpose, whereas dialkylamino and alkoxy groups according to Rizzardo and co-workers are less adequate 31. Additionally, R 1 should be a good free radical leaving group compared to the propagating radicals, and capable to re-initiate free radical polymerisation. Groups like CH 2 -Ar, CH 2 -C=C, CH 2 -C=, CH 2 -CCN and others, in conjugation to the radical, are appropriate to stabilise for mesomeric reasons, whereas stabilisation due to inductive effects can be achieved by the use of alkyl groups 50. In Figure 2.11 the proposed mechanism for RAFT polymerisation is presented 11. I R (1) R monomer kp RMn (2) RMn + Z S S S R 1 Z S MnR + R1 (3) RMm + Z S S MnR ktr Z S S MmR + RMn (4) RMm + RMn RMm RMn (dead polymer chain) (5) Figure 2.11: Transfer polymerisation. Proposed mechanism for the Reversible Addition-Fragmentation chain As shown above, polymerisation process initiates by the radicals formed due to decomposition of the initiator I (step 1). Subsequently, the propagating radicals (step 2) react with CTA molecules resulting to the formation of dormant chains (transferred chains) and radical leaving groups R 1 (step 3). The latter are capable of initiating another chain. Hence, the amount of radicals remains constant during the whole process.
21 INTRDUCTIN Functionalised polymers with metal complexing segments ver the past three decades many examples appeared in the literature, where macromolecular science seems to be strongly oriented towards the field of organic-inorganic hybrid materials 2,51,52. A combination of potential applications of metal compounds with the special properties of polymers can lead to the formation of nanometer-scale structured materials with for example good mechanical performance and electrosteric stabilisation of colloids 53. Coordination polymers with -, S-, and N-containing ligands and their ability to form polymer-metal complexes with different metal ions have been extensively investigated. Antonietti and co-workers 54 have synthesised novel amphiphilic block copolymers with nitrogen, sulfur and phosphonate moieties, which make them suitable for complexation and solubilisation of different transition-metal ions in organic media. More precisely, they have shown that the functionalised block copolymers form micelles in organic solvents. Those micellar solutions are used for solubilising diverse transition-metal salts such as Cu(Cl 4 ) 2, Pd(CH 3 C) 2, ZnCl 2, Rh(CH 3 C) 2 etc. which are otherwise insoluble. Furthermore, addition of a reducing agent in the solutions of metal salt-containing micelles, leads to the formation of well-defined noble metal colloids. Chernyshov et al. 55 have prepared a new type of a chelating block copolymer with triphenylphosphine groups (Figure 2.12). Those groups are well known for their widespread use in coordination chemistry and catalysis 56. x y Ph 2 P Figure 2.12: Polystyrene-block-poly-m-vinyltriphenylphosphine (ps-b-pph). Complexation of these polymers with palladium compounds results in the formation of spherical aggregates, presumably uni- and multi-lamellar vesicles and disk-like micelles. Additionally, block copolymer-stabilised Pd nanoparticles were prepared by reduction of the
22 INTRDUCTIN 16 Pd-containing ps-b-pph block copolymer micellar aggregates using different reducing reagents. Schubert and co-workers have a number of publications on functionalised polymers with metal-complexing segments such as bi- and terpyridine. ne example is the synthesis of linear oligomers and polymers with two terpyridine end-groups 57. Complexation with transition-metal ions results in the formation of non-covalent coordination polymers (Figure 2.13). n n Figure 2.13: Schematic representation of the proposed non-covalent polymerisation induced by complexation of terpyridine functionalised telechelics with transition metal ions 57. In another publication, they reported the introduction of mono- and difunctionalised 6,6 dimethyl-2,2`-bipyridines into polyesters, aiming to design polymeric biodegradable architectures with specific metal binding units 58. Furthermore, they have developed a new strategy, giving rise to metallo-supramolecular block copolymers. In such polymers, a metal/ligand complex serves as a supramolecular linker between the hydrophobic and hydrophilic blocks of the amphiphilic block copolymers. For example, a metallosupramolecular poly(styrene)-block-poly(ethylene oxide) was prepared via self-organisation of the α-methoxy-ω-(2,2`:6`,2``-terpyridinyl)oxypoly(ethylene oxide)ruthenium(iii) complex and ω-(2,2`:6`,2``-terpyridine)oxypoly(styrene) (ps-[ru]pe) 59. This polymer has the ability to form micelles in water with a PS core surrounded by bis(2,2`:6`,2``terpyridine)ruthenium(ii) complexes and a pe corona. The same principle was applied for the synthesis of metallo-supramolecular graft copolymers 60. The well-known strong affinity of bidentate β-dicarbonyl moieties to multivalent cations 61 prompted some groups to synthesise polymers with β-dicarbonyl repeating units (Figure 2.14). So far, such polymers have been obtained by free radical polymerisation of methacroylacetone 62, ethyl (meth)acrylolylacetate 63 and 2-(acetoacetoxy)ethyl methacrylate 64 or by the controlled oxidation of poly(vinyl alcohol) 65.